1524 S.J. Lim et al. / Thin Solid Films 516 (2008) 1523–1528
2. Experimental details
A homemade transverse flow type ALD reactor was used for
ALD of ZnO thin films. Fig. 1 is a schematic drawing of ALD
system. Substrate is heated by halogen lamp located outside of
quartz tube chamber body, providing growth temperature up to
500 °C. DEZ, Epichem adduct grade, was used as a metal
precursor and water vapor without bubbling was used as a
reactant. Ar was used as a purging and carrier gas, whose inlet
was separated at the side of the chamber. The Ar flow was
controlled by mass flow controller (5.5 sccm for DEZ bubbler
and 60 sccm for purging). For constant flowing of water, the
temperature of water container was maintained at 65 °C. DEZ
bubbler temperature was maintained at 13 °C by using a cooling
circulator, producing vapor pressure of 1066 Pa. To prevent
possible problems caused by the very high pressure of DEZ, the
bubbler pressure was set to 5.46 × 104 Pa by using Ar. The flows
of precursor and reactant were controlled by needle valve to set
the pressure of the reactor to 40 Pa for water and 17.3 Pa for
DEZ flowing step. ALD ZnO films were deposited at the
growth temperature range from 100 °C to 250 °C. Typical ALD
ZnO growth sequence is composed of 2 s of DEZ exposure, 8 s
of Ar purging, 3 s of H2O exposure, and 4 s of Ar purging.
Typically, the number of ALD cycles was 200 times.
The sputtering system is equipped with three sputter guns,
two DCs and one rf, enabling co-sputtering. For this work, rf
sputtering was used by using 5.06-cm-diameter ZnO target with
99.99% purity. The distance from the target to the substrate was Fig. 2. Growth rates of thermal ALD ZnO prepared at Ts = 200 °C on Si(001) as a
9.5 cm and the base pressure was 6.66 × 10− 4 Pa. Deposition function of (a) DEZ exposure time (ts) and (b) water exposure time (tr).
was conducted at room temperature with varying sputtering
power (50, 100, and 150 W) and working pressure (0.2, 0.67, for 1 min. The thickness was routinely measured by ellipsometer
and 1.33 Pa). The substrate was rotated with 20–25 rpm during (Rudolph auto ELII). The microstructures of the ZnO films were
film deposition and pre-sputtering was conducted before analyzed by X-ray diffraction (XRD) and cross-sectional
deposition to remove contamination on target surface. transmission electron microscopy (JEOL, model JEM2010F).
The substrates were corning glass 1737 and Si(001) substrate. X-ray photoemission spectroscopy (XPS) was used for deter-
While the glass substrates were cleaned by consequential mining composition of ZnO films. For XPS, specimens were
dipping in trichloroethylene, acetone, and methanol, respective- cleaned by Ar sputtering in situ for 4–5 nm in XPS chamber
ly, for 10 min, the Si substrates were cleaned by degreasing using before measurement, and energy scan was carried out at around
acetone, IPA, and water followed by dipping in 1% HF solution O 1s, Zn 2p3/2, and C 1s position with monochromatic AlKα
radiation source. The resistivity was routinely measured by a 4-
point probe. Resistivity of ZnO was measured by 2-point probe
method using Keithley 6517 electrometer when Samples have
resistance Over 20 GΩ. For this measurement, we deposited Al
through shadow mask to fabricate electrodes with various widths
and lengths to eliminate the effects of contact resistance. Hall
measurements were carried out for samples with resistivity
lower than 20 GΩ. Hall measurement system was HL5500PC
(Accent Optical Technologies) at Material Characterization
Center in Korea Photonics Technology Institute.
3. Experimental results
3.1. ZnO deposition: ALD and sputtering
Fig. 2a shows the growth rates of ALD ZnO thin films, usually
represented by thickness/cycle, as a function of DEZ exposure
Fig. 1. Schematic drawing of hot wall type thermal ALD setup. time (ts) at Ts = 200 °C on Si(001) substrates. No difference in
S.J. Lim et al. / Thin Solid Films 516 (2008) 1523–1528 1525
probably due to the incomplete surface reaction . However,
when the surface reaction is not limited by the surface reaction
of precursor, the surface hydroxyl density, acting as an
adsorption site for precursors, determines the growth rate.
Thus, at high growth temperature region, the surface hydroxyl
density decreases with increasing growth temperature leading to
reduction in the growth rate.
The XRD spectra of ALD ZnO thin films grown on glass
substrates at growth temperatures between 100 and 250 °C are
shown in Fig. 4. For all the samples, XRD spectra show that
ALD ZnO films are composed of hexagonal wurtzite structure
grains with strong (002) diffraction peak, implying that most of
the c-axis of ZnO grains are arranged perpendicular to the
Fig. 3. Growth rates of thermal ALD ZnO on Si(001) as a function of growth
growth rate was observed for glass substrate. The growth rate
increases with increasing ts and saturates at ∼1.7 Å/cycle at
ts N 2 s. The saturation of growth rate indicates that a typical ALD
mode growth is achieved by self-limited adsorption of DEZ at
200 °C. This growth rate is almost 0.3 Å/cycle higher than the
previously reported value (1.4 Å/cycle)  and almost same as
that of another report (1.65–1.7 Å/cycle) . The growth rate
change with water exposure time (tr) also shows good saturation at
tr N 3 s (Fig. 2b). From the thickness vs. the number of growth
cycles data (not shown), almost no nucleation delay was observed
on Si(001) and glass substrate.
In Fig. 3, the growth rates of ALD ZnO as a function of
growth temperature are shown between Ts = 100 and 250 °C.
The growth rates increase with increasing temperatures at low
growth temperature, reaching highest value of 2.0 Å/cycle at
175 °C. Above 175 °C, the growth rates decrease again to
1.12 Å/cycle at 250 °C. Similar trends were reported for ALD
ZnO from DEZ and water [22,25]. This seems to be a typical
behavior for ALD oxides from alkyl precursor and water. For
example, ALD of Al2O3 from trimethyl aluminum and water,
which has been intensively studied, shows almost same
behavior [26,27]. At low growth temperature regions, the
growth rate decreases with decreasing growth temperature
Fig. 4. XRD spectra of ALD ZnO thin films on glass prepared at different Fig. 5. XPS spectra of ALD ZnO thin films prepared at Ts = 200 °C on Si(001)
growth temperatures. showing binding energy range of (a) Zn 2p3/2, (b) O 1s, and (c) C 1s.
1526 S.J. Lim et al. / Thin Solid Films 516 (2008) 1523–1528
substrate surface. However, (002) peak is especially dominant at
high temperature over 175 °C. In several previous reports, (100)
preferred orientation was usually observed for ALD ZnO at low
growth temperatures [21–23]. However, (002) preferred
orientation was reported to become stronger with increasing
growth temperatures [22,25]. In fact, the preferred orientation of
ALD ZnO has been reported to be largely dependent upon
growth conditions. For example, (002) was the smallest for
photo ALD  and addition of O2 changes the preferred
orientation from (100) to (002) .
Chemical bonding states and impurity contents in the films
were investigated by XPS. Fig. 5 shows the XPS spectra of
ALD ZnO film with thickness of 350 Å, prepared at 200 °C on
Fig. 7. XRD spectra of rf sputtered ZnO films prepared at 100 W, 0.2 Pa and
silicon substrate. The sample was sputter-cleaned in situ right
150 W, 1.33 Pa.
before the XPS measurement. The Zn 2p spectrum shown in
Fig. 5a indicates that the peak position agrees well with the
binding energy of Zn 2p3/2 from wurtzite ZnO phase, reported to constant, while at a high pressure of 1.33 Pa, it increases almost
be at 1022.4 eV  and the experimental data were well fitted monotonically with increasing rf power. The growth rate during rf
with single Gaussian peak. No metallic Zn at 1021.5 eV was sputtering is determined by the sputtering yield, target to substrate
observed, indicating that all Zn atoms are in Zn2 state . The distance, and scattering of sputtered species. The exact reason for
O 1s spectrum shown in Fig. 4b is composed of single this complicated behavior of the growth rate dependence shown in
component peak at 531.05 eV, which is associated with O2 ions Fig. 6 is not clearly understood yet.
in oxygen deficient state . Same O 1s peak position was ZnO films prepared by rf sputtering at all sputtering powers
reported for metal organic CVD ZnO from DEZ and O2 . and working pressures show strong (002) preferred orientation
No additional peak related to O2 from excessive O2 (533.3 eV) (Fig. 7). Predominant (002) preferred orientation for room
or O–H bonding (532.3 eV) was observed as a higher energy temperature rf sputtered ZnO is a general observation .
side tail [30,33]. Especially, no C contaminant was observed Compared to the ALD ZnO in Fig. 4, the sputtered ZnO seems
within detection limit of XPS (∼ 1%), which would have been
observed at 284.6 eV (Fig. 5c). So ALD ZnO produced in the
current study is quite pure.
For comparison, ZnO thin films were deposited at room
temperature by rf sputtering on Si (001) and glass substrates. The
measured thicknesses of sputtered ZnO films are plotted in Fig. 6
as a function of rf sputtering power (from 50 to 150 W) for three
different Ar pressure (0.2, 0.67, and 1.33 Pa) for 20 min of the
total deposition time. Overall, the growth rates increase with
increasing rf power since the number of atoms sputtered from the
target increases with rf power. But the trend of growth rate change
largely depends on the operating pressure. At low Ar pressure of
0.2 Pa, the growth rate increases up to 100 W, then remains almost
Fig. 6. Growth rate of rf sputtered ZnO as a function of sputtering power at
working pressures of 0.2, 0.67, and 1.33 Pa. The depositions were done at room Fig. 8. (a) Resistivity and (b) mobility and carrier concentration of ALD ZnO on
temperature. glass as a function of growth temperature.
S.J. Lim et al. / Thin Solid Films 516 (2008) 1523–1528 1527
to have more predominant (002) preferred orientation judging values were reported in previous reports for undoped ALD ZnO
from the existence of small additional peaks for ALD ZnO. In films [22,25]. However, the resistivity increases with decreasing
contrast to a previous report showing amorphous phase growth temperature, reaching 23.5 Ω cm at Ts = 100 °C.
formation at high sputtering power , we did not observe Especially at Ts = 125 °C, relatively high hall mobility (15 cm2/
any amorphous film formation within all the investigated V s) with low carrier concentration, 4.1× 1017 cm− 3, was
deposition parameter ranges. However, at 150 W sputtering obtained. In a previous report , the increase in resistivity
power and under 1.33 Pa, small (101) and (110) diffraction with the decrease in mobility and carrier concentration was
peaks were also observed, indicating the microstructure is observed with decreasing growth temperature below 140 °C,
weakly dependent on growth parameters for rf sputtering of which is similar to our results . However, in another report
ZnO. from ozone as a reactant, the opposite trend was observed at
higher growth temperature region above 240 °C .
3.2. Comparisons of electrical properties Fig. 9a is resistivity measurement results of rf sputtered ZnO
thin films on glass at Ts = room temperature. In this case, since
Room temperature electrical resistivity, carrier mobility, and all the films were deposited at room temperature, the data are
carrier concentration were measured for both ALD and sputtered plotted as a function of rf sputtering power and operating
ZnO. The results of ALD ZnO thin films on glass substrates pressure. At all Ar pressure studied, the resistivity values were
prepared at various growth temperatures are shown in Fig. 8. All measured to be high at 50 and 100 W. For these cases, the Hall
the ALD ZnO thin films show n-type conductivity by Hall measurements could not be done due to too large resistivity.
measurement system, agreeing with all previous studies on ZnO Overall, the resistivity was above 1 kΩ cm, with highest values
ALD [21,22,24,25]. Due to n-type carriers, the ALD ZnO films, of almost 10 MΩ cm at 100 W, 0.2 Pa pressure. The carrier
even without any intentional doping, show relatively high mobility and concentrations were measured for only the
conductivity. Fig. 8a shows that the resistivity at Ts N 150 °C is samples deposited at 150 W and plotted as a function of
low at around 0.012–0.04 Ω cm. This relatively low resistivity operating pressures. With small variations, the mobility was
can be attributed to the high mobility (13.5–20 cm2/V s) and around 1.5–3.3 cm 2 /V s with carrier concentrations of
carrier concentration (1–3.7 × 1019 cm− 3) in the films. Similar 4 × 1019 cm− 3 to 2 × 1020 cm− 3 range with n-type conductivity.
Although we could not measure the carrier concentrations and
mobilities for the films deposited at 50 and 100 W, the carrier
concentrations should be very small estimated from almost 5 to
8 orders of magnitude higher resistivity than those at 150 W,
since the mobility difference should not be very large.
Until now, the exact physical origin for n-type conductivity in
ZnO is not known. Most plausibly, the origin of n-type
conduction is the inherent defects in the film such as oxygen
vacancies or interstitial Zn atoms. However, other possibility
due to H impurity in the films cannot be excluded . Usually,
the low carrier concentration is expected to result in high
mobility, which is contrary to the current observations for ALD
ZnO. The single crystal ZnO can exhibit very high mobility up to
300 cm2/V s . Thus, the low mobility of polycrystalline ZnO
thin films has been often attributed to the Schottky barrier at the
grain boundary. In other words, the charges trapped at the grain
boundaries make high-energy barrier for carrier transport,
producing low mobility. So although the carrier concentration
is low and the mobility inside the grain may be high for ALD
ZnO films prepared at low growth temperatures, the existence of
high-energy barrier at grain boundary seems to result in this low
mobility. In contrast, the relatively small number of charges
trapped at grain boundary results in higher mobility for ZnO
films at higher growth temperature, although the carrier
concentration is high. The exact reason for this difference in
grain boundary energy barrier depending on growth temperature
Fig. 9. (a) Resistivity as a function of sputtering power and (b) hall mobility and is not understood yet. One possibility is that more impurities are
carrier concentration as a function of working pressure for rf sputtered ZnO on gathered at grain boundaries at lower growth temperature,
glass prepared at room temperature. leading to lower mobility.
1528 S.J. Lim et al. / Thin Solid Films 516 (2008) 1523–1528
Meanwhile, the sputtered ZnO thin films prepared at 50–100 W Acknowledgements
rf sputtering power should have very small inherent defect
concentration, judging from very high resistivity at these growth This work was supported by Samsung SDI, POSTECH Core
conditions. However, the films deposited at high power have low Research Program, Korean Research Foundation Grant funded by
resistivity with high carrier concentrations. One possible explana- the Korean Government(MOEHRD)(KRF-2005-005-J13102),
tion for this observation is that inherent defects are prone to be and POSRIP. The authors are deeply thankful to Prof. Wang
generated at high sputtering power due to the arrival of energetic Chul Zin for help in ellipsometry analysis.
depositing particles, leading to higher carrier concentration.
However, considering that the sputtered power used in the present References
study is not that high, more plausible reason may be that the
inherent defects creation is thermodynamically preferable. Thus,  S.P.S. Arya, O.N. Srivastava, Cryst. Res. Technol. 23 (1988) 669.
kinetically controlled deposition environment at lower sputtering  J.K. Srivastava, L. Agrawal, B. Bhattacharyya, J. Electrochem. Soc. 11
power produces films with lower carrier concentrations. (1989) 3414.
 Z.C. Jin, C.G. Granqvist, Proc. SPIE 21 (1987) 827.
For application as an active channel layer of TTFT, ZnO thin  C. Lee, K. Lim, J. Song, Sol. Energy Mater. Sol. Cells 43 (1996) 37.
film should have high mobility. In this regard, the ALD ZnO  S.J. Pearton, D.P. Norton, K. Ip, Y.W. Heo, T. Steiner, Prog. Mater. Sci. 50
prepared at 175 °C, which has highest mobility, has great (2005) 293.
benefits. But the Hall measurements indicate that these films  H.S. Bae, S. Im, Thin Solid Films 469 (2004) 75.
have too high carrier concentration. This high carrier concen-  S.K. Hazra, S. Basu, Solid State Electron. 49 (2005) 1158.
 S. Muthukumar, C.R. Gorla, N.W. Emanetoglu, S. Liang, Y. Lu, J. Cryst.
tration will contribute to large off current. Considering that the Growth 225 (2001) 197.
on–off current ratio of active layer should be at least 106, these  V. Assuncao, E. Fortunato, A. Marques, H. Aguas, I. Ferreira, M.E.V.
films may not be good for TFT applications. In this regard, the Costa, R. Martins, Thin Solid Films 427 (2003) 401.
ALD ZnO films deposited at low concentration with relatively  S. Jager, B. Szyszka, J. Szczyrbowski, G. Bauer, Surf. Coat. Technol. 98
low off current may be better for TFT applications, while they
 E. Fortunato, P. Barquinha, A. Pimentel, A. Gonçalves, A. Marques, L.
could suffer from low mobility. All these results indicate that the Pereira, R. Martins, Thin Solid Films 487 (2005) 205.
ALD process should be properly modified for fabricating ZnO  H. Cheng, C. Chen, C. Lee, Thin Solid Films 498 (2006) 142.
active layers for TFT fabrication. These include changes in  R.L. Hoffman, J. Appl. Phys. 95 (2004) 5813.
reactants and precursors, the use of radical-based ALD, or  P. Barquinha, E. Fortunato, A. Gonçalves, A. Pimentel, A. Marques, L.
proper doping of extra elements. For example, much lower Pereira, R. Martins, Superlattices Microstruct. 39 (2006) 319.
 E. Fortunato, P. Barguinha, A. Pimentel, A. Gonçalves, A. Marques, L.
carrier concentrations were observed for O3-based ZnO ALD Pereira, R. Martins, Adv. Mater. 17 (2005) 590.
. Sputtered ZnO, especially at low rf sputtering powers,  P.F. Carcia, R.S. McLean, M.H. Reilly, G. Nunes Jr., Appl. Phys. Lett. 82
seems more promising for TFT applications at this stage. Using (2003) 1117.
similar growth techniques, TTFT with reasonably good  S. Masuda, K. Kitamura, Y. Okumura, S. Miyatake, J. Appl. Phys. 93
characteristics was fabricated using these kinds of high- (2003) 1624.
 Y. Ohyam, T. Niwa, T. Ban, Y. Takahashi, Jpn. J. Appl. Phys. 297 (2001)
resistivity ZnO films in the previous reports . However, 40.
with the absence of device characteristics using the ZnO films  A.N. Banerjee, C.K. Ghosh, K.K. Chattopadhyay, H. Minoura, A. Sarkar,
prepared in this study, decisive predictions cannot be done at A. Akiba, A. Kamiya, T. Endo, Thin Solid Films 496 (2006) 112.
this time. Modifications of ALD and sputtering processes are  H. Kim, J. Vac. Sci. Technol., B 21 (2003) 2231.
currently under investigation. Initial results seem promising,  A. Yamada, B. Sang, M. Konagai, Appl. Surf. Sci. 112 (1997) 216.
 V. Lujala, J. Skarp, M. Tammenmaa, T. Suntola, Appl. Surf. Sci. 82–83
indicating that electrical properties can be tuned by changing (1994) 34.
key growth parameters.  E. Yousfi, J. Fouache, D. Lincot, Appl. Surf. Sci. 153 (2000) 223.
 A.W. Ott, R.P.H. Chang, Mater. Chem. Phys. 58 (1999) 132.
5. Conclusions  S.K. Kim, C.S. Hwang, S. Ko Park, S.J. Yun, Thin Solid Films 478 (2005)
 R. Matero, A. Rhatu, M. Ritala, M. Leskela, T. Sajavaara, Thin Solid Films
ZnO thin films were prepared by thermal ALD and rf 368 (2000) 1.
sputtering technique at low growth temperatures. XPS results of  R.L. Pruunen, J. Appl. Phys. 97 (2005) 121301.
ALD ZnO show no carbon contamination in the films without  Y. Yamamoto, K. Saito, K. Takahashi, M. Konagai, Sol. Energy Mater. Sol.
O–H bond. Both ALD and sputtered ZnO thin films have Cells 65 (2001) 125.
 S.-H. Ko Park, Y.E. Lee, J. Mater. Sci. 39 (2004) 2195.
generally (002) preferred orientations, while more predominant
 M. Islam, T.B. Glosh, K.L. Chopra, H.N. Acharya, Thin Solid Films 280
c-axis preferred orientation was observed in sputtering. The (1996) 20.
electrical properties of ZnO films were found to be largely  M. Chen, X. Wang, Y.H. Yu, Z.L. Pei, X.D. Bai, C. Sun, R.F. Huang, L.S.
dependent on growth parameters. For ALD ZnO, resistivity Wen, Appl. Surf. Sci. 158 (2000) 134.
changes up to two orders of magnitude were observed depending  Y. Zhang, G. Du, X. Wang, W. Li, X. Yang, Y. Ma, B. Zhao, H. Yang, D.
on growth temperatures. The sputtered ZnO films have shown Liu, S. Yang, J. Cryst. Growth 252 (2003) 180.
 B.J. Coppa, R.F. Davis, Appl. Phys. Lett. 82 (2003) 400.
resistivities spanning over 9 orders of magnitude depending on  Z. Zhou, K. Kato, T. Komaki, M. Yoshino, H. Yakawa, M. Morinaga, Int.
sputtering power. Due to relatively high carrier concentrations in J. Hydrogen Energy 29 (2004) 323.
ALD ZnO, proper modifications in deposition process should be  Ü. Özgür, I. Alivov, C. Liu, A. Teke, M.A. Reshchikov, S. Dogan, V.
carried out to be used as an active channel layer in TFT. Avrutin, S.-J. Cho, H. Mokoç, J. Appl. Phys. 98 (2005) 041301.